Macromolecules 1994,27, 7938-7940
Stereospecific Polymerization of Methyl Methacrylate Initiated by DimethylzirconocenelB(C$F& (or P~CB(C~FS).I)/Z~(C~H)Z
promotes the polymerization of MMA in the presence of Zn(C2H& at ambient temperature in toluene. A chiral racemic zirconocene compound, ruc-EtEIndIzZr(CH3)2, gave highly isotactic PMMA, while an achiral zirconocene,Cpzzr(C&)z, gave syndio-richatactic PMMA. This paper reports the preliminary results of these polymerizations. Results and Discussion. Addition of B(CsF5)3 ( 1 ) or Ph&B(CsF5)4 (2) and equimolar CpzZr(CH& (3) into a toluene solution of MMA could not initiate polymerization of MMA. Under these conditions metallocene cationic complexes (e.g., CpzZr(CH3)+B(CsF5)4-) are formed in high yield. When MMA was at first mixed with Zn(C2Hs)z in a toluene solvent and aged for 1 h before subsequent addition of compounds 1 and 3 (see the Experimental Part), however, polymerizations were initiated to give PMMAs with high molecular weight and narrow molecular mass distributions in good yields. Some complexes were formed between MMA and Zn(C2H5)2, which were indicated by a downfield shift of carbonyl of MMA from 167.7 to 167.9 ppm and an upfield shift of methylene protons of Zn(CzH5)z from 7.2 to 7.0 ppm observed in the 13C NMR spectrum after aging. It was confirmed from a 13CNMR spectrum that no polymerization occurred until final addition of zirconocene. In this condition, however, almost no polymer could be obtained when CH2C12 was used as the solvent, which was reported as a good solvent for the polymerization of MMA with the CpzZr(CH3)(THF)+BPb-/CpzZr(CH3)2 c a t a l y ~ t . ~The results of polymerizations conducted in toluene are summarized in Table 1. The 13CNMR spectrum of a typical polymer is displayed in Figure 1,whereas the pentad distributions are shown in Table 2, both of which indicate that PMMA produced with CpzZr(CH& is a syndio-rich atactic polymer. The microtacticity distributions of the polymer were found to obey Bernoullian statistics (Table 2), suggesting that
Kazuo Soga,* Hai Deng, Takuya Yano, and Takeshi Shiono Research Laboratory of Resources Utilization, Tokyo Institute of Technology, 4259 Nagatsuta, Midori-ku, Yokohama 227, Japan Received April 29, 1994 Revised Manuscript Received October 14, 1994
Stereospecificpolymerization of methyl methacrylate (MMA) has been intensively investigated in anionic polymerizations initiated by lithium alkyls or Grignard reagents. Both isotactic and syndiotactic poly(methy1 methacrylate) (PMMA) can be produced, but only a t very low temperatures.l Recently, much attention was focused on lanthanocene hydride and alkyl compounds, which polymerize olefins2without any cocatalyst in high yields and also produce syndiotactic PMMA3 with very narrow molecular mass distributions at ambient temperatures. Cationic metallocene compounds of the Group 4 elements, which have similar electronic structures, have attracted more attention due to high activity and high stereospecificity in olefin p~lymerization.~ It has been recently reported that a cationic zirconocene compound, Cp2Zr(CH3)(THF)+BPh4-, promotes syndiospecific polymerization of MMA in the presence of neutral zirconocene (Cp$r(CH3)2),5a and a substoichiometric mixture (ca. 1:3)of [nBwNHI[BPbl and ruc- or (S)-(+)-Et(H11nd)zZr(CH3)2gives isotactic PMMA in polar solvent like C H ~ C ~ Z . ~ ~ More recently, we have found that the catalyst composed of a dimethylzirconocene compound and a stoichiometric amount of Lewis acid like B(C&"5)3
H3C0, F=O mm
d b C
w PP* I
Figure 1. 13C NMR spectrum of atactic poly(MMA) obtained in run no. 7 (Table 1).
0024-9297/94/2227-7938$04.50/00 1994 American Chemical Society
Communications to the Editor 7939
Macromolecules, Vol. 27, No. 26, 1994
d b C
NMR spectrum of isotactic poly(MMA) obtained in run no. 2 (Table 1).
the syndiospecific polymerization proceeds via a chain end-controlled mechanism. Similar results have been reported with the lanthanocene3 and CpzZrCH3(THF)+BP~*-/CP~Z~(CH catalysts. &~ On the other hand, the 13C NMR spectrum of PMMA produced with rac-Et[Indl2Zr(CH& is shown in Figure 2, which is an isospecific catalyst in, e.g., the polymerization of propylene. From the spectrum, together with the analytical results listed in Table 2, it is clear that the polymer is highly isotactic, with a high molecular weight and a broader molecular mass distribution. The intensity ratios of [mmmrl:[mmrrl:[mrrml pentads were found to be approximately 2:2:1. Therefore, isotactic polymerization proceeds via an enantiomorphic sitecontrolled mechanism, which is completely different from the chain end-controlled mechanism in isotactic polymerization of MMA with Grignard reagents in to1uene.l The remarkable feature of this catalyst system is that the isotactic selectivity was very high (the selectivity of one prochiral face on the enantiomorphic site: /3 = 0.99) even a t a temperature as high as 40 "C, which indicates that the isotactic propagation site is very stable in the presence of Zn(C2Hs)z. Furthermore, the glass transition temperature (T,)of the isotactic PMMA measured by DSC was about 55.0 & 2.5 "C,which
is very close to the theoretical value calculated previously.6 We also attempted to employ (iPr)FluCpZr(CH3)2to polymerize MMA, which is a syndiospecific catalyst in the polymerization of propylene. But no polymer was obtained under the conditions shown in Table 1. While the dependence of stereoselectivity on zirconocene was described above, the effect of zinc compounds was also investigated by using the Cp2Zr(CH3)2/ B(C&'5)3 system. Use of Zn(CH& or Zd(CH2hCH-CH212 only resulted in a trace amount of PMMA, of which the structure was similar to that obtained by Zn(C2Hd2. Besides Zn(CzH&, stronger Lewis acids like B(C2Hd3 and N(C2H5)3 were used as well; however, the polymerization could not be induced. Further study is in progress to investigate the role of Zn(CzH5)z as well as the mechanism of polymerization, the results of which will be reported elsewhere. Experimental Part. MMA monomer and toluene were dried over calcium hydride and distilled before use. (iPr)B(CGF&,~C P ~ Z ~ ( C Hru~-Et[IndI2Zr(CHd2,~ ~)~,~ FluCpZr(CH3)2,1°Zn(CH3)211were synthesized according to the literature. Zn[(CH2)2CH=CH& was synthesized from a stoichiometric mixture of the Grignard reagent
Table 1. Polymerization Results of MMA" run no. 1 2 3
4 5 6 7 8 9
catalyst Et(Ind)zZr(CHj)z/lor 2 Et(Ind)zZr(CH~)$l Et(Ind)zZr(CH3)~/2 Et(Ind)-~Zr(CH3)$1 CpzZr(CH3)$1 or 2 CpzZr(CHdd1 CpzZr(CHs)z/l CpzZr(CHdzi1 (iPr)FluCpZr(CHa)z/l or 2
[Zn(CzH&l (mM) 0
214 214 214 0 8.18 214 214 214
temp ("C) 0 0 0
40 0 0 0
40 0 or 40
yieldb (%) 0 38 37 23 0 26 64 8
23.2 29.0 15.2
1.78 1.62 1.70
52.8 57.6 54.5
103 48.2 12.6
1.25 1.38 1.85
128 128 122
Polymerization conditions: [Zr] = 0.227 mM; 1, B(C6F&; 2,PhaC(C6Fd.r; [ l ] =  = 0.227 mM, [=I = 0.85 M, toluene = 13.3mL for 24 h. * Yield = weight of polymer obtaineuweight of monomer used. c Measured by GPC calibrated with standard polystyrene samples. a
7940 Communications to the Editor 5 I/
Macromolecules, Vol. 27, No. 26, 1994
and ZnClz. Zn(CzH& and Ph3CB(C6F5)4 were donated from Tosoh Akzo Co. Ltd. The other chemicals were research grade and were purchased from commercial sources and used without further purification. Polymerization of MMA was carried out under a dry nitrogen atmosphere in a 100-mLround-bottomed flask equipped with a magnetic stirrer. A typical polymerization process is as follows: toluene (13.3 mL), MMA (2.0 mL), and a 1.0 M heptane solution of Zn(C2Hs)z (4.7 mL) were injected into the flask, and the mixture was stirred for 1h at 0 "C. After the addition of a 5.0 mM toluene solution of B(CeF& (1.0 mL), a 5.0 mM toluene solution of CpzZr(CH3)z (1.0 mL) was immediately injected to start the polymerization. The polymerization was quenched at 0 "C with methanol mixed with hydrochloric acid. The polymer produced was precipitated into methanol, followed by drying in vacuo at 60 "C for 8 h. The molecular weight and molecular mass distribution were measured by GPC (Shimazu 9A) at room temperature using chloroform as the solvent and calibrated with standard polystyrene samples. The glass transition temperature (T,)was measured with a Seiko DSC-220C calorimeter at a heating rate of 10 "C/min. The 13C NMR spectra were measured in chloroform-d at room temperature with a JEOL GX-270 NMR spectrometer. Broad-band decoupling was used to remove the 13C-lH coupling. The center peak of chloroform-d was used as the internal reference (77.0 ppm).
References and Notes Hatada, K; Kitayama, T.; Ute, K. Prog. Polym. Sci. 1988, 13, 189 and references therein. (a) Jeske, G.; Lauke, H.; Mauermann, H.; Sepson, P. N.; Schumann, H.; Marks, T. J.; J.Am. Chem. SOC.1985,107, 8091. (b) Watson, P. L.; Parshall, G. W. ACC.Chem. Res. 1986,18, 51. (c) Coughlin, B.; Barcow, J . E. J . Am. Chem. SOC.1992, 114, 7606. (a) Yasuda, H.; Yamamoto, H.; Yokota, K.; Miyake, S.; Nakamura, A. J. Am. Chem. SOC.1992, 114, 4908. (b) Yasuda, H.; Yamamoto, H.; Yamashita, M. Macromolecules 1993,26, 7134. For example: (a)Hlatky, G. G.; Turner, H. W.; Echman, R. R. J.Am. Chem. SOC.1989,111,2728. (b)Jeshuis, J.; Tan, Y. Y.; Teuben, J. H. J.Mol. Catal. 1990,62,277. (c) Yang, X.; Stern,C. L.; Marks, T. J. J.Am. Chem. SOC.1991,113, 3623. (d) Ewen, J. A.; Elder, M. J.;Jones, R. L.; Haspeslagh, L.; Atwood, J. L.; Bott,S. G.; Robinson, K. Makromol. Chem., Macromol. Symp. 1991,48149, 253.
(a) Collins, S.; Ward, D. G. J. Am. Chem. SOC.1992, 114, 5460. (b) Collins, S.; Ward, D. G. Abst. Pup., Am. Chem. SOC.1992, IN-354. Thompson, E. V. J. Polym. Sci., Polym. Phys. Ed. 1966, 4 , 199. Massey, A. G.; Park, A. J. J. Organomet. Chem. 1964, 2, 245. Wailes, P. C.; Weigold, H.; Bell, A. P. J. Organomet. Chem. 1972, 34, 155. Samuel, E.; Rausch, M. D. J . Am. Chem. SOC.1973,95, 6263. Chien, J. C. W.; Tsai, W. M.; Rausch, M. D. J.Am. Chem. SOC.1991,113,8570. Ewen, J. A.; Jones, R. L.; Razavi, A.; Ferrara, J . D. J.Am. Chem. SOC.1988,110, 5255. Gray, A. P.; Callear, A. B.; Edgecornbe, F. H. C. Can. J . Chem. 1963,41, 152.